Fracture-mechanics parameters of the composite-enamel bond.
In a previous study, the critical values of the opening mode stress intensity factor (K1), its equivalent, the strain energy-release rate (G1), and the J integral (J1) (in the elastic case being equal to that of G1) were determined for resin composite. In this study, the strength of the composite-tooth interface was investigated. The critical values of K1 and J1 were measured with single-edge notched-bend (SENB) specimens of resin composite bonded to enamel, with the notch at midspan at the bonded interface. Due to enamel's anisotropy, the values of Klc and Jlc to be used in a fracture-mechanics application for failure prediction of a structure depend on the enamel prism orientation relative to the adhesive interface. Where interfacial failure is to be expected, the following values for Jlc and Klc can be used: Silux, Jlc = 145 +/- 35 Jm-2 and Klc = 0.84 +/- 0.16 MNm-3/2; P-30, Jlc = 163 +/- 13 Jm-2 and Klc = 1.02 +/- 0.07 MNm-3/2. Where enamel failure is expected or where the failure mode cannot be predicted, the following values can be applied: Silux, Jlc = 89 +/- 15 Jm-2 and Klc = 0.84 +/- 0.16 MNm-3/2; P-30, Jlc = 89 +/- 15 Jm-2 and Klc = 0.75 +/- 0.10 MNm-3/2.
Department of Cariology and Endodontology, School of Dentistry, University of Nijmegen, The Netherlands.
R
R
de Groot
H C
HC
van Elst
M C
MC
Peters
D003188:Composite Resins; D001840:Dental Bonding; D003743:Dental Enamel; D003799:Dental Stress Analysis; D006801:Humans; D008855:Microscopy, Electron, Scanning
D003188:Composite Resins